LMucko/crystallography-open-database huggingface dataset:
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht005_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003337
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht005_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.114 Ca2 Fe1.886 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.4217
_cell_length_b                   14.7432
_cell_length_c                   5.5960
_cell_formula_units_Z            4
_cell_volume                     447.306
_database_code_amcsd             0003426
_exptl_crystal_density_diffrn    3.988
_cod_original_formula_sum        'Ca2 (Fe1.886 Al.114) O5'
_cod_database_code               9003337
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht015_1
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003338
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht015_1
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.204 Ca2 Fe1.796 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.4140
_cell_length_b                   14.7163
_cell_length_c                   5.5947
_cell_volume                     445.752
_cell_formula_units_Z            4
_database_code_amcsd             0003427
_exptl_crystal_density_diffrn    3.963
_cod_original_formula_sum        'Ca2 (Fe1.796 Al.204) O5'
_cod_database_code               9003338
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht025_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003339
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht025_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.276 Ca2 Fe1.724 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.4071
_cell_length_b                   14.6949
_cell_length_c                   5.5941
_cell_volume                     444.489
_cell_formula_units_Z            4
_database_code_amcsd             0003428
_exptl_crystal_density_diffrn    3.943
_cod_original_formula_sum        'Ca2 (Fe1.724 Al.276) O5'
_cod_database_code               9003339
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht030_3
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003340
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht030_3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.365 Ca2 Fe1.635 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.4027
_cell_length_b                   14.6779
_cell_length_c                   5.5923
_cell_volume                     443.471
_cell_formula_units_Z            4
_database_code_amcsd             0003429
_exptl_crystal_density_diffrn    3.914
_cod_original_formula_sum        'Ca2 (Fe1.635 Al.365) O5'
_cod_database_code               9003340
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht035_1
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003341
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht035_1
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.408 Ca2 Fe1.592 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3986
_cell_length_b                   14.6631
_cell_length_c                   5.5910
_cell_volume                     442.585
_cell_formula_units_Z            4
_database_code_amcsd             0003430
_exptl_crystal_density_diffrn    3.903
_cod_original_formula_sum        'Ca2 (Fe1.592 Al.408) O5'
_cod_database_code               9003341
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht040_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003342
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht040_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.441 Ca2 Fe1.559 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3936
_cell_length_b                   14.6476
_cell_length_c                   5.5899
_cell_volume                     441.621
_cell_formula_units_Z            4
_database_code_amcsd             0003431
_exptl_crystal_density_diffrn    3.897
_cod_original_formula_sum        'Ca2 (Fe1.559 Al.441) O5'
_cod_database_code               9003342
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bf80i_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003343
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bf80i_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.46 Ca2 Fe1.54 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3876
_cell_length_b                   14.6302
_cell_length_c                   5.5877
_cell_volume                     440.432
_cell_formula_units_Z            4
_database_code_amcsd             0003432
_exptl_crystal_density_diffrn    3.899
_cod_original_formula_sum        'Ca2 (Fe1.54 Al.46) O5'
_cod_database_code               9003343
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht55_1
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003344
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht55_1
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.552 Ca2 Fe1.448 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3808
_cell_length_b                   14.6131
_cell_length_c                   5.5911
_cell_volume                     439.629
_cell_formula_units_Z            4
_database_code_amcsd             0003433
_exptl_crystal_density_diffrn    3.866
_cod_original_formula_sum        'Ca2 (Fe1.448 Al.552) O5'
_cod_database_code               9003344
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht50_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003345
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht50_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.59 Ca2 Fe1.41 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3832
_cell_length_b                   14.6214
_cell_length_c                   5.5916
_cell_volume                     440.114
_cell_formula_units_Z            4
_database_code_amcsd             0003434
_exptl_crystal_density_diffrn    3.846
_cod_original_formula_sum        'Ca2 (Fe1.41 Al.59) O5'
_cod_database_code               9003345
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht070_1
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003346
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht070_1
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.663 Ca2 Fe1.337 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3714
_cell_length_b                   14.5805
_cell_length_c                   5.5847
_cell_volume                     437.381
_cell_formula_units_Z            4
_database_code_amcsd             0003435
_exptl_crystal_density_diffrn    3.838
_cod_original_formula_sum        'Ca2 (Fe1.337 Al.663) O5'
_cod_database_code               9003346
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht120_6
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003347
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht120_6
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.789 Ca2 Fe1.211 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3569
_cell_length_b                   14.5407
_cell_length_c                   5.5735
_cell_volume                     434.137
_cell_formula_units_Z            4
_database_code_amcsd             0003436
_exptl_crystal_density_diffrn    3.811
_cod_original_formula_sum        'Ca2 (Fe1.211 Al.789) O5'
_cod_database_code               9003347
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht095_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003348
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht095_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.866 Ca2 Fe1.134 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3510
_cell_length_b                   14.5256
_cell_length_c                   5.5685
_cell_volume                     432.820
_cell_formula_units_Z            4
_database_code_amcsd             0003437
_exptl_crystal_density_diffrn    3.788
_cod_original_formula_sum        'Ca2 (Fe1.134 Al.866) O5'
_cod_database_code               9003348
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht100_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003349
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht100_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.909 Ca2 Fe1.091 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3469
_cell_length_b                   14.5149
_cell_length_c                   5.5640
_cell_volume                     431.820
_cell_formula_units_Z            4
_database_code_amcsd             0003438
_exptl_crystal_density_diffrn    3.778
_cod_original_formula_sum        'Ca2 (Fe1.091 Al.909) O5'
_cod_database_code               9003349
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht110n1
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003350
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht110n1
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al0.986 Ca2 Fe1.014 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3369
_cell_length_b                   14.4945
_cell_length_c                   5.5548
_cell_volume                     429.695
_cell_formula_units_Z            4
_database_code_amcsd             0003439
_exptl_crystal_density_diffrn    3.762
_cod_original_formula_sum        'Ca2 (Fe1.014 Al.986) O5'
_cod_database_code               9003350
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht120n2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003351
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht120n2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al1.078 Ca2 Fe0.922 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3269
_cell_length_b                   14.4687
_cell_length_c                   5.5433
_cell_volume                     427.241
_cell_formula_units_Z            4
_database_code_amcsd             0003440
_exptl_crystal_density_diffrn    3.743
_cod_original_formula_sum        'Ca2 (Fe.922 Al1.078) O5'
_cod_database_code               9003351
Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5: Single-crystal X-ray diffraction at 25 deg C and high temperature X-ray powder diffraction (25 C <= T <= 1000 C) Sample: bht130_2
Redhammer, G. J.; Tippelt, G.; Roth, G.; Amthauer, G.; American Mineralogist 89 (2004) 405–420; doi:

data_9003352
_publ_section_title
;
 Structural variations in the brownmillerite series Ca2(Fe2-xAlx)O5:
 Single-crystal X-ray diffraction at 25 deg C and high temperature
 X-ray powder diffraction (25 C <= T <= 1000 C)
 Sample: bht130_2
;
_journal_name_full               'American Mineralogist'
_journal_page_first              405
_journal_page_last               420
_journal_volume                  89
_journal_year                    2004
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al1.259 Ca2 Fe0.741 O5'
_chemical_name_mineral           Brownmillerite
_space_group_IT_number           46
_symmetry_space_group_name_Hall  'I -2b 2'
_symmetry_space_group_name_H-M   'I 2 m b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.3093
_cell_length_b                   14.4534
_cell_length_c                   5.5230
_cell_volume                     423.821
_cell_formula_units_Z            4
_database_code_amcsd             0003441
_exptl_crystal_density_diffrn    3.691
_cod_original_formula_sum        'Ca2 (Fe.741 Al1.259) O5'
_cod_database_code               9003352